interface studies by second-harmonic generation studies by second-harmonic generation during...
Post on 11-Jun-2018
Embed Size (px)
Interface studies by second-harmonic generation during silicon-based materials processing
PROEFSCHRIFT ter verkrijging van de graad van doctor aan de Technische Universiteit Eindhoven, op gezag van de Rector Magnificus, prof.dr.ir. C.J. van Duijn, voor een commissie aangewezen door het College voor Promoties in het openbaar te verdedigen op maandag 16 juni 2008 om 16.00 uur door Joost Jozef Hendrik Gielis geboren te Weert
Dit proefschrift is goedgekeurd door de promotor: prof.dr.ir. M.C.M. van de Sanden Copromotor: dr.ir. W.M.M. Kessels The work presented in this thesis is part of the research project Dynamics of plasma-activated surface processes (99TF24), which is financially supported by the Netherlands Foundation for Fundamental Research on Matter (FOM). Printed and bound by: Printservice Technische Universiteit Eindhoven. Cover: Mirror Lake, Yosemite National Park, CA, USA (photograph: Joost Gielis). Cover design: Oranje Vormgevers, Eindhoven. CIP-DATA LIBRARY TECHNISCHE UNIVERSITEIT EINDHOVEN Gielis, Joost Jozef Hendrik Interface studies by second-harmonic generation during silicon-based materials processing / by Joost Jozef Hendrik Gielis. Eindhoven : Technische Universiteit Eindhoven, 2008. Proefschrift. ISBN 978-90-386-1286-7 NUR 926 Trefwoorden: niet-lineaire optica / amorf silicium / siliciumoppervlakken / dunnelaagfabricage / ellipsometrie / infraroodspectroscopie Subject headings: second-harmonic generation / amorphous silicon / silicon / surface states / thin films / plasma materials processing / ellipsometry / infrared spectroscopy
PREFACE In this thesis the application of the surface and interface sensitive nonlinear optical technique of second-harmonic generation during silicon-based materials processing is explored. The thesis is divided into seven chapters. Chapter 1 describes the framework in which the research has been performed, as well as the motivation of the research and the approach chosen. Furthermore, the key results and conclusions are presented in this chapter. Chapters 2-7 consist of separate articles that have been published or will be published in international scientific journals. More specifically, in Chapter 2 aspects relevant for the application of second-harmonic generation in thin film geometries are described, providing a theoretical and experimental background for the rest of the thesis. In Chapters 3-7 the results obtained in various areas of silicon-based materials processing are presented in detail.
Joost Gielis Eindhoven, April 2008
CONTENTS Chapter 1 Framework and overview of the research
Chapter 2 Optical second-harmonic generation in thin film systems In preparation for publication: J.J.H. Gielis, P.M. Gevers, I.M.P. Aarts, M.C.M. van de Sanden, and W.M.M. Kessels.
Chapter 3 Spectroscopic second-harmonic generation during Ar+-ion bombardment of Si(100) Published as: J.J.H. Gielis, P.M. Gevers, A.A.E. Stevens, H.C.W. Beijerinck, M.C.M. van de Sanden, and W.M.M. Kessels, Phys. Rev. B 74, 165311 (2006).
Chapter 4 a-Si:H/c-Si heterointerface formation and epitaxial growth studied by real-time optical probes Published as: J.J.H. Gielis, P.J. van den Oever, M.C.M. van de Sanden, and W.M.M. Kessels, Appl. Phys. Lett. 90, 202108 (2007).
Chapter 5 Real-time study of a-Si:H/c-Si heterointerface formation and epitaxial Si growth by spectroscopic ellipsometry, infrared spectroscopy and second-harmonic generation Accepted for publication in Phys. Rev. B: J.J.H. Gielis, P.J. van den Oever, B. Hoex, M.C.M. van de Sanden, and W.M.M. Kessels.
Chapter 6 Negative charge and charging dynamics in Al2O3 films on Si characterized by second-harmonic generation Submitted for publication: J.J.H. Gielis, B. Hoex, M.C.M. van de Sanden, and W.M.M. Kessels.
Chapter 7 Second-harmonic spectroscopy of Si nanocrystals embedded in silica Accepted for publication in Phys. Stat. Sol. (c): A. Wirth, J. Wei, J.J.H. Gielis, P. Figliozzi, J. Rafaelsen, Y.Q. An, and M.C. Downer.
List of publications related to this work
Chapter 1 Framework and overview of the research
I. INTRODUCTION TO SILICON-BASED MATERIALS PROCESSING Silicon technology is one of the cornerstones of present day society. Almost all means of computation, data storage and communication rely on silicon-based microelectronics. Integrated circuits (ICs) of electronic devices, such as complementary metal-oxide-semiconductor (CMOS) field-effect transistors, patterned on silicon substrates do not only form the heart of every computer, they are, for example, also the processing core of cellular phones and provide the engine management of modern cars. Volatile memory devices such as dynamic random access memory (DRAM) and nonvolatile memory for mobile applications such as flash memory, as well as transceiver ICs that enable wireless and mobile communication are based on silicon technology. The nearly endless list of applications also includes optoelectronic devices such as flat panel thin film transistor (TFT) displays and charged couple devices (CCD) used in digital cameras, as well as upcoming devices such as photonic crystals and microelectromechanical systems (MEMS). Silicon also plays a dominant role in photovoltaics. Over 90% of the market share consists of wafer-based crystalline silicon (c-Si) and multicrystalline Si solar cells, whereas both amorphous and crystalline Si thin film solar cell concepts are emerging. The photovoltaic market has been growing at an average rate of 35% per year since 1998, which is a trend that will continue in the next years.1 Since 2006 the worldwide consumption of Si by the photovoltaic industry even exceeds the amount consumed by the microelectronics industry.2 In Fig. 1 several silicon-based devices are illustrated. For all these applications of silicon technology a clear common trend is visible: critical device dimensions are continuously decreasing. In microelectronics this trend is known as Moores Law, stating a doubling of the number density of electronic components approximately every 24 months.5 Formulated in 1965 this law is still valid, and nowadays this law even dictates the semiconductor roadmap.6 Decreasing dimensions in photovoltaics manifest themselves for example by the cost-driven reduction of overall solar cell thickness, the application of thinner layers (e.g., the emitter), and the increasing importance of thin-film-based solar cell concepts. Due to the miniaturization the surface-to-volume ratio increases, yielding an increasing importance of surface and interface properties on the performance of actual devices. Surfaces and interfaces do not only have different characteristics compared to the corresponding bulk material, these regions are often also relatively defect-rich, which can adversely affect device performance. Another phenomenon of the downscaling is the need for alternative materials, either as a replacement for materials that reached the limit of their scalability or because a new functionality is required. The introduction of other materials inherently induces new interface characteristics. In addition to their direct
Framework and overview of the research
impact on device performance, surfaces and interfaces are the active regions during materials processing. In this thesis surface and interface aspects will be studied during silicon-based materials processing. Different relevant areas of Si-based materials processing will be addressed, such as (1) the etching of micro- and nanostructures in Si; (2) the deposition of Si thin films; (3) the introduction of new materials such as Al2O3 thin films; and (4) the implementation of novel Si-based device technologies. We will start by introducing these areas in more detail. A. Silicon etching The etching of silicon or silicon-based materials is an important processing step in the creation of micro- and nanostructures as required in many of the aforementioned examples such as DRAM, CMOS, MEMS and photonic crystals [cf. Figs 1(a)-1(d)]. Generally, the substrate is coated prior to
5 nm Silicon
(a) (b) (c)
FIG. 1 Various applications of silicon technology: (a) Deep trenches etched in Si forDRAM applications [Qimonda]. The trenches are 4.4 m deep and ~100 nm wide. (b) 45 nm dual-core processor die [Intel]. (c) Transistor based on 45 nm technology with high- (Hf-based) dielectric and metal gate [Intel]. (d) MEMS multiple gear reductiondevice etched in Si [Sandia National Laboratories]. (e) Hydrogenated amorphous Si (a-Si:H)/crystalline Si heterojunction used in Si heterojunction solar cells.3,4 (f) Si heterojunction solar cell power plant, Sesma, Spain [Sanyo].
etching with a photosensitive resist that is exposed to light through a patterned mask. Subsequently, the illuminated part of the resist is removed and the pattern is etched in the underlying silicon. For the etching step two different techniques can be used: wet chemical etching and plasma etching. Plasma etching, also referred to as dry etching, has an important advantage
Si OAl H
C F ion
FIG. 2 (a) Schematic and simplified illustration of trench etching in c-Si by a CF4/Ar plasma. The ions and the etchants induce a synergetic effect that enhances the etchrate and the anisotropy of the process. The amor